LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS

 Marlene Walton
 8 months ago
 Views:
Transcription
1 XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds it all together. A corresponding and related lamination theory for the strength of laminates would be equally important and useful. It would complete the understanding of the behavior of fiber composite materials in its most important and prime form of usage, laminates. This research report extends the technical program established in Ref. [1]. In that work Christenen and Lonkar [1] developed failure criteria that were mainly intended for quasiisotropic fiber composite laminates. This work develops the much broader and much more generally useful failure criteria for wide classes of orthotropic fiber composite laminates. The quasiisotropic laminates case is important because it is one limiting case of fiber composite laminations. The other limiting case is the unidirectional form itself. The class of orthotropy supplies the general and inclusive bridge of cases in between and including these two limiting cases. General cases such as these have been treated in the large and highly publicized composites failure program of Hinton and Kaddour [2]. The end result of that program served more to show the utter and unrelenting complexity of the overall problem rather than providing any unified and directly applicable results. The following work will begin by recalling some previous results from Ref. [1] and then pursuing a very large scale extension of the method. This will allow the treatment of the general case of orthotropic laminates where the degree of anisotropy in the plane of the laminate can be arbitrarily specified as necessary for a very wide range of layup patterns and problem specifications. At the lamina level the fiber composites form will be taken as highly anisotropic, appropriate to very high stiffness and high strength fibers (typified by carbon fibers) in a polymeric matrix. It will be found that the failure criteria for the general orthotropic laminate is completely calibrated by only two fiber dominated failure properties at the unidirectional lamina or the tow level of the fibermatrix
2 system. Calibrating the failure theory for general orthotropic laminates by use of only two failure properties certainly would have been thought to be impossible. This seemingly intractable problem will be solved here, removing a large obstacle to meaningful fiber composites applications. The case of unidirectional fiber composites failure was treated in Ref. [3]. As already discussed, the complementary case of the failure of quasiisotropic laminates was treated in Ref. [1]. Associated with these two works, then the present work completes the longstanding task by rigorously treating the failure of a very wide class of orthotropic laminates. This new work on composites failure could equally well be presented in a mechanics oriented materials journal or a composite materials journal. The application is to composites but the methodology is totally mechanics based. This development would not be possible were it not for the insight and avenues of approach opened up by only the mechanics discipline. The usual composites failure approach zeroes in on one particular failure mechanism and treats that in some, usually great detail. The mechanics approach used here is much broader and more inclusive, but not at the expense of rigor. The present approach will be found to be satisfyingly rigorous and general The primary reason for conducting this research and writing this paper is to provide a viable tool for use with computational mechanics. Composites research sources seem to be preoccupied with other matters and not interested in pursuing the general failure problem. Perhaps the failure problem is considered by them to be too difficult or even impossibly difficult. Nevertheless the problem desperately needs attention, solution, and subsequent application. This work accepts the challenge to produce general failure results so that computational mechanics can then take over and open up new directions for the applications of fiber composite materials. Orthotropic Laminates Failure Theory In Ref. [1] Christensen and Lonkar derived the failure criterion for quasiisotropic laminates. It was shown to have the same form as that for threedimensionally isotropic materials when in the 2D state of plane stress. It is given by 1 T 1 C σ T 1 C σ TC σ σ 11 σ 22 + σ TC σ (1)
3 where T and C are the uniaxial strengths of the laminate. Now rewrite this in slightly modified but equivalent form that will be helpful in the following orthotropic developments, as given by 1 T 1 C σ T 1 C σ σ 11 TC σ 11 TC σ 22 TC + σ 22 TC TC σ (2) In Ref. [1] the quasiisotropic form in (2) was shown to generalize to the failure criterion for orthotropic laminates in plane stress as 1 1 σ T 22 σ 22 + C 11 σ 11 C 11 2 C 22 σ 11 σ 22 C 11 T 22 C 22 + σ 22 T 22 C σ S 12 (3) where, C 11, T 22, C 22 are the tensile and compressive strengths in the 1 and 2 stress directions and S 12 is the shear strength. The orthotropic form given in Ref. [1] appears a little different from that in (3) but it is equivalent. These five calibrating strengths are directly measurable from standard, single stress component 1D tests. Form (3) is remarkably simple for the failure criterion of fully and generally orthotropic laminates. It will be developed even much further in the following derivation. For these further developments, temporarily return to the case of the quasiisotropic laminate, as treated in Ref. [1]. The failure criterion (1) only requires two strength properties to completely calibrate it. These are the uniaxial tensile and compressive strengths T and C. In a special development in Ref. [1] it was shown that the uniaxial strengths T and C for the laminate can be expressed in terms of the unidirectional fiber composites tow strengths as T = T tow 3 (4) and
4 C = C tow 3 (5) These are physically realistic approximations that apply for fiber dominated systems. The term fiber dominated means that the fibers are greatly stiffer and stronger than is the surrounding polymeric matrix phase of the composite material. In effect then the fiber phase is a completely one dimensional reinforcing agent, meaning that the fiber contribution to the stiffness and strength of the laminate is purely through its unidirectional, axial direction contribution. A slightly more complicated quasiisotropic form than (5) for the compressive strength property was derived in Ref. [1]. The simpler form (5) will be used here. It is here considered that the form in Ref. [1] is more appropriate for use with the unidirectional compressive strength being obtained from a very thin lamina form allowing the kink band mechanism of failure whereas the form (5) is more appropriate for use when the unidirectional compressive strength as determined from a monolithic type test specimen. The form (5) will be used here as being representative of the compressive strength obtained directly from the impregnated fiber tow as manufactured rather than from the further processed lamina form. Next the fiber dominated forms (4) and (5) for the quasiisotropic case will be generalized for use with the orthotropic case. This will be found to be a major and completing step forward in understanding general composites laminate strength behavior. The orthotropic laminate will be taken as the standard 0, 90, ± 45 degree layup pattern as shown in Fig. 1.
5 Fig. 1 Lamination pattern Take c 0, c 45, c 45, and c 90 as the specified volume fractions of the four lamina orientations in the orthotropic laminate. For orthotropic symmetry it is required that Thus it follows that c 45 = c 45 (6) c 0 + 2c 45 + c 90 = 1 (7) The objective here is the generalization for fiber dominated systems from the quasiisotropic case (4) and (5) to the orthotropic case. The five calibrating strengths, C 11, T 22, C 22, and S 12 will now be derived in terms of the general volume fractions c 0, c 90, and c 45 and they will be left open to later specification for particular cases. First consider the shear strength S 12. For the fiber dominated system the 0 and 90 plies make no contribution to the shear strength, only the 45 plies give shear resistance. Furthermore the shear strength must be proportional to the volume of
6 the active material in shear deformation and thus must be linearly dependent on c 45. Then take S 12 = αc 45 T tow C tow (8) where α is an unknown coefficient to be determined. The dependence shown in (8) on T tow and C tow follows from the quasiisotropic form for S from (1) as S = TC 3 = 1 3 T tow C tow 3 (9) Lastly parameter α in (8) at c 45 = ¼ then requires α = (10) to recover the form in (9). This completes the determination of orthotropic S 12. The other 4 cases for the uniaxial strengths are considerably more complex to determine. Before proceeding to the next cases it should be noted that this fiber dominated approach can give some strength properties as being zero. For example, if there were no ± 45 plies then the shear strength (8) would vanish. Of course this just would mean that the failure is totally matrix controlled and would be of very low strength capability compared with the fiber dominated and controlled failure modes. This would further mean that this would be a very poor design and should be discarded. The path to be followed for the determination of, C 11, T 22, C 22 is exactly like that of the classical lamination theory used with stiffness. But instead of stiffness, strength will be the determining factor. With stiffness the lamination theory procedure usually requires a computer to keep account of the bookkeeping for the tensor transformations. But for the fiber dominated strength problem the procedure is much simpler since the fibers are one dimensional load bearing members. In fact it is rather intriguing to watch the theory unfold and lead to surprisingly simple and clear results. First for the determination of the uniaxial strength take a unit strain in the direction. This induces a strain and consequently a fiber direction stress in the ± 45
7 lamina, for these fiber dominated lamina. Now resolve this c 45 stress into the coordinate axes directions using the tensor transformations. For no transverse stress in the laminate to exist, the 2 direction stress in the ± 45 lamina must be resisted by the 90 degree lamina. This leads to the determination of the orthotropic Poisson s ratio ν 12 as Similarly it is found that ν 12 = ν 21 = c 90 c 45 (11) c 0 c 45 (12) When c 45 = 0 then from (11) and (12) ν 12 = ν 21 = 0 as must be the case for the fiber dominated system in a crossply laminate. When c 90 = 0 in (11) then ν 12 = 1 meaning that there is no resistance to lateral strain change. Similarly when c 0 = 0 in (12). Finally the resolution of all the fiber direction stresses into the 1 direction gives the uniaxial tensile strength in that direction as Similarly it can be derived that and = c 0 + c 45c 90 c c 90 T tow (13) C 11 = c 0 + c 45c 90 c c 90 C tow (14) T 22 = c 90 + c c 45 0 c c 0 T tow (15)
8 C 22 = c 90 + c 45c 0 c c 0 C tow (16) The completing shear strength from (8) and (10) is given by S 12 = 4c 45 3 T tow C tow 3 (17) Relations (13)(17) are the full strength properties needed to calibrate the general orthotropic failure criterion (3). They also are of great interest in their own right for an orthotropic laminate. The uniaxial strengths (13)  (16) can also be written in terms of the Poisson s ratios in the compact forms where ν 12 and ν 21 are given by (11) and (12). = ( c 0 +ν 12 c 90 )T tow (18) C 11 = ( c 0 +ν 12 c 90 )C tow (19) T 22 = ( c 90 +ν 21 c 0 )T tow (20) C 22 = ( c 90 +ν 21 c 0 )C tow (21) The basic relations (3) and (13) (17) are powerful results. Not only do they represent the solution to a previously unsolved, very important problem, they do so in an exceedingly simple, clear and concise form. They comprise the orthotropic lamination theory for the strength of fiber dominated composite materials. Contrary to the author s initial and cursory expectation, this much more complex problem and solution is fully as rigorous as the specialized quasiisotropic results in [1]. They include the quasiisotropic forms as a special case. The uniaxial and shear strengths (13) (17) satisfy all the necessary consistency tests. These are as follows. First note that for a unidirectional lamina (13) gives = T tow as must occur. The strengths (13) (17) also have the necessary forms for a fiber dominated crossply laminate necessarily having no shear resistence. The complementary case of only ± 45 s shows the scissoring effect with no resistance
9 that must occur. Finally, when relations (13) (17) are reduced to the quasiisotropic case by taking c 0 = c 90 = c 45 = 1/ 4 the correct quasiisotropic results are recovered from (13) (17), namely (4) and (5). This fiber dominated orthotropic failure theory can be derived for any orthotropic laminate, not just for 0, 90, ± 45 laminates. The forms are a little more complex, but entirely manageable. Such results will be presented in due course. But the 0, 90, ± 45 case is the most important and the simplest case and the one that completely and naturally conforms to orthotropic symmetry. It is emphasized here. The five strengths in (13) (17) are entirely specified by only the two tow strengths for any orthotropic, 0, 90, ± 45 layup. Of course this result is restricted to fiber dominated systems such as carbon fiber, polymeric matrix composites. The enabling operation for this unexpected development is that these five calibrating properties for the orthotropic case are only one dimensional problems. In these cases one can reason which lamina orientations in the four directions are applicable for fiber dominated systems and which are inapplicable for each of the five properties. This operation could not be accomplished if it involved biaxial stress conditions. Effectively critical strain in the 1D fiber direction specifies the failure condition in the uniaxial cases aligned with the symmetry axes. It should be emphasized that fiber dominated systems cannot sustain all stress states. For example for c ±45 = 0 then (13) (15) cannot support a shear stress state. But this simply means that the matrix phase controls failure for such a condition. That would be of no interest for fiber composites. The fiber dominated state must be designed to support the load under all anticipated loading conditions. The final and complete statement of failure criteria for orthotropic laminates is given by the failure criterion (3) with the five calibrating strengths specified by (13) (17) as expressed in terms of the two tow strength properties. To imagine that the complete strength specification for any stress state in the orthotropic laminate could be specified from only two experimental measurements would have seemed impossible before the derivation in this paper.
10 A Specific Example and General Failure Results Everything up to this point up to this point has been motivated and necessitated by original research. Now some interesting consequences from the general theory will be developed and then used in an example. Full blown design procedures for failure would normally involve investigating many different states of stress that could occur in practice. The simplest possible problem of this type will be opened here by prescribing the allowable stress states for the two uniaxial tensile stresses and for the shear stress, taken as individual conditions. After that the more general case will be taken up. As a simple but realistic example take the volume fractions of the lamina orientations as c 0 = 4 7 (22) c 90 = c 45 = 1 7 Thus in terms of volume fractions the anisotropy ratio is c 0 c 90 = 4 (23) From (13) (17) it follows that the tensile uniaxial and shear strengths are given by = T tow T 22 = T tow (24) S 12 = 4 21 T tow C tow 3 With similar forms for C 11 and C 22.
11 From (24) the anisotropy ratio in strengths has the value T 22 = 3 (25) Thus the degree of strength anisotropy is a little less than the anisotropy ratio in the volume fractions (23) but both are highly anisotropic in this example. To go further with a general example take realistic tow strengths for IM7 like carbon fiber polymeric matrix unidirectional strength properties as T tow = 2700 MPa C tow = 1700 MPa (26) For the orthotropic laminate specified by the volume fractions (22) the condition is effectively that of 4/7 of the lamina being in a quasiisotropic arrangement with the additional 3/7 of the lamina added to the 0 direction lamina. The uniaxial and shear strengths are then given by = 1671 MPa C 11 = 1052 T 22 = 557 (27) C 22 = 351 S 12 = 236 The corresponding quasiisotropic problem properties are given by T = 900 MPa C = 567 (28) S = 412
12 Finally the quasiisotropic properties (28) are put into the failure criterion (1) and the orthotropic properties (27) are put into the orthotropic failure criterion (3) giving the resulting failure envelopes shown in Fig. 2, with σ 12 taken as zero. Fig. 2 Failure for fiber dominated unidirectional, intermediate, and quasiisotropic laminates Also shown in Fig. 2 is the representation of the unidirectional tow properties given by (26). Fig. 2 graphically and dramatically shows the progression starting from the unidirectional fiber composites strengths going to and through an intermediate form and finally coming to the other limiting case, the quasiisotropic form. This fiber dominated formalism would not be expected to be realistic near the unidirectional limiting case since it does not include the transverse matrix controlled effects. Other than the need for the micro scale matrix controlled properties the present failure theory applies to and for all orthotropic layup patterns. Complete and comprehensive design applications would involve trade offs between specification of the volume fractions for the four fiber orientations using the lamination rules (13) (17) and then the failure criterion (3). Unsatisfactory
13 results would then require further iteration. Using all this in a numerical program for analysis of an entire structure would complete the process. For this to occur efficiently and effectively it would require a sophisticated numerical algorithm. This new lamination/strength theory provides the vital link in the whole process. With regard to applications and design for applications, it would not be appropriate to use the present fiber dominated methodology for problems having any of the three lamina volume fractions near zero. That condition would require some explicit account of the matrix properties. Also, in any actual application it would always be necessary to have experimental certification of the general results. Further Verification of the Orthotropic Failure Criterion Quasiisotropic laminates are a special case of orthotropic laminates. The previous verification with test results was given in Ref. [1] for the quasiisotropic case. That comparison was for a biaxial spread of data, mainly in the range of compressivecompressive stresses for the principal stresses applied to the laminate. The present verification will involve the state of uniaxial tensile stress at failure. The rationale behind the derivation of the formulas (4) and (5) relating tow failure properties to uniaxial laminate failure properties is as follows. In the tow type failure specimen the strain at failure is given by ε f = T tow E tow (29) where E tow is the elastic modulus of the impregnated tow material. In the quasiisotropic laminate at failure the strain in the lamina that first fails is taken to be the same strain as occurs in the tow specimen. So then for the quasiisotropic laminate in uniaxial tensile stress T E = ε f (30) with E being the laminate elastic modulus. Thus from (29) and (30) T E = T tow E tow (31)
14 Rearranging (31) gives T T tow = E E tow (32) From (32) it follows that if E/E tow = 1/3 can be proven from testing data then it further follows that T/T tow = 1/3 thus verifying (4). Similar arguments would follow for the compressive case of (5). It is much easier and more reliable to measure nondestructive elastic properties than it is to measure failure properties. Thus the proof of E = E tow /3 for the quasiisotropic laminate will suffice to prove (4) and (5). The elastic properties for a quasiisotropic laminate have been quite exhaustively measured by Van Otterloo and Dayal [4]. The values for the elastic modulus E were measured by both ultrasound and mechanical means in 11 different directions in the layup. The mean value for E from the 22 tests was E = 58.5 GPa Measured (33) If only ultrasound data were used the mean was 63.1 GPa. The corresponding modulus of the tow material was measured as E tow = GPa. Using the formula E E tow = 1 3 (34) which is from Ref. [1], Eq. (31), with E 11 = E tow for the fiber dominated system then gives E = 59.5 GPa Predicted (35) Thus the comparison of (33) and (35) provides the further verification of the failure theory.
15 The Next Step The basic research problem of the development of failure theory for fiber composite laminates has now been completed and consummated. This does not however terminate interest in the problem. It actually represents the beginning of a new phase to be used in the applications of fiber composite materials. A major step in that direction will be to develop a complete and comprehensive design methodology for fiber composite laminates. Using the results of this paper, this consolidation will be given in a subsequent paper and it will involve both the stiffness and the strength of fiber composite laminates in a form directly appropriate for applications. References 1. Christensen, R. M., and Lonkar, K., (2017), Failure Theory/Failure Criteria for Fiber Composite Laminates, J. Appl. Mech., 84, Hinton, M. J., and Kaddour, A. S., (2013), The Second WorldWide Failure Exercise Part B, J. Composite Materials, 47, Christensen, R. M., (2014), Completion and Closure on Failure Criteria for Unidirectional Fiber Composite Materials, J. Appl. Mech., 81, Van Otterloo, D. L., and Dayal, V., (2003), How Isotropic are Quasi Isotropic Laminates, Composites Part A: Applied Science and Manufacturing, 34, Richard M. Christensen June 9 th, 2017 Copyright 2017 Richard M. Christensen
QUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More information9 Strength Theories of Lamina
9 trength Theories of Lamina 9 TRENGTH O ORTHOTROPIC LAMINA or isotropic materials the simplest method to predict failure is to compare the applied stresses to the strengths or some other allowable stresses.
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationAnalysis of high loss viscoelastic composites
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationVI. CRITICAL EXPERIMENTAL AND THEORETICAL TESTS FOR FAILURE CRITERIA
VI. CRITICAL EXPERIMENTAL AND THEORETICAL TESTS FOR FAILURE CRITERIA The term critical tests implies more than just a routine comparison with some convenient data. First, a candidate failure criterion
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationGeology 229 Engineering Geology. Lecture 5. Engineering Properties of Rocks (West, Ch. 6)
Geology 229 Engineering Geology Lecture 5 Engineering Properties of Rocks (West, Ch. 6) Common mechanic properties: Density; Elastic properties:  elastic modulii Outline of this Lecture 1. Uniaxial rock
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationDESIGN OF COMPOSITE LAMINATED STRUCTURES BY POLAR METHOD AND TOPOLOGY OPTIMISATION
DESIGN OF COMPOSIE LAMINAED SUCUES BY POLA MEOD AND OPOLOGY OPIMISAION A. Jibawy,,3, C. Julien,,3, B. Desmorat,,4, (*), A. Vincenti UPMC Univ Paris 6, UM 79, Institut Jean Le ond d Alembert B.P. 6 4, place
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationA New Ultrasonic Immersion Technique to Retrieve Anisotropic Stiffness Matrix for Dispersion Curves Algorithms
A New Ultrasonic Immersion Technique to Retrieve Anisotropic Stiffness Matrix for Dispersion Curves Algorithms DARUN BARAZANCHY 1, WILLIAM ROTH 2 and VICTOR GIURGIUTIU 3 ABSTRACT Dispersion curve algorithms
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationCORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS
CORRELATING OFFAXIS TENSION TESTS TO SHEAR MODULUS OF WOODBASED PANELS By Edmond P. Saliklis 1 and Robert H. Falk ABSTRACT: The weakness of existing relationships correlating offaxis modulus of elasticity
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationMECHANICS OF MATERIALS. EQUATIONS AND THEOREMS
1 MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS Version 20110114 Stress tensor Definition of traction vector (1) Cauchy theorem (2) Equilibrium (3) Invariants (4) (5) (6) or, written in terms of principal
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationPLY WAVINESS ON INPLANE STIFFNESS OF COMPOSITE LAMINATES
PLY WAVINESS ON INPLANE STIFFNESS OF COMPOSITE LAMINATES Cimini Jr., Carlos A., and Tsai, Stephen W. 2 Department of Mechanical Engineering, Federal University of Minas Gerais Av. Antônio Carlos, 6627
More informationStacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous Orthotropic Laminates.
49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials 710 April 2008, Schaumburg, IL AIAA 20081940 Stacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationThe Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
11th European Conference on NonDestructive Testing (ECNDT 214), October 61, 214, Prague, Czech Republic The Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationUsing MATLAB to Design and Analyse Composite Laminates
Engineering, 2010, 2, 904916 doi:10.4236/eng.2010.211114 Published Online November 2010 (http://www.scirp.org/journal/eng). Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop,
More informationBuckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate
Buckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate Outline Introduction Representative Volume Element (RVE) Periodic Boundary Conditions on RVE Homogenization Method Analytical
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationOverview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling
Overview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling R. Haynes epartment of erospace Engineering, Georgia Institute of Technology 27 Ferst rive W, tlanta, G 33325, US robert.haynes@gatech.edu
More informationFatigue Failure Criteria for Unidirectional Fiber Composites 1
Z. Hashin 2 Professor and Chairman, Department ol Solid Mechanics, Materials and Structures, Tel Aviv University, RamatAvlv, Tel Aviv 69978, Israel. Fellow ASME Fatigue Failure Criteria for Unidirectional
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationFLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION N. V. De Carvalho 1*, B. Y. Chen
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationA CRITERION OF TENSILE FAILURE FOR HYPERELASTIC MATERIALS AND ITS APPLICATION TO VISCOELASTICVISCOPLASTIC MATERIALS
MTS ADHESIVES PROGRAMME 19961999 PERFORMANCE OF ADHESIVE JOINTS Project: PAJ1; Failure Criteria and their Application to ViscoElastic/ViscoPlastic Materials Report 2 A CRITERION OF TENSILE FAILURE FOR
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationMultiple SpatioTemporal Scale Modeling of Composites Subjected to Cyclic Loading
Multiple SpatioTemporal Scale Modeling of Composites Subjected to Cyclic Loading Robert Crouch 1, Caglar Oskay 1, and Stephen Clay 2 1 Department of Civil and Environmental Engineering, Vanderbilt University,
More informationFailure Mode Predictions in the Compressive Response of Laminated Composites
Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA
More informationJeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA UNESCO EOLSS
MECHANICS OF MATERIALS Jeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA Keywords: Solid mechanics, stress, strain, yield strength Contents 1. Introduction 2. Stress
More information3dimensional joint torque calculation of compression sportswear using 3DCG human model
3dimensional joint torque calculation of compression sportswear using 3DCG human model Akihiro Matsuda, University of Tsukuba Hirokazu Tanaka, University of Tsukuba Hitoshi Aoki, University of Tsukuba
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationAspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites
Aspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites J.A.Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Abstract A fiber s efficiency in a
More informationMECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS
MECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS This paper provides a preliminary stress analysis of a carbon reinforced layered cylinder such as would be found in a yacht mast. The cylinder is
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationMODELING OF CONCRETE MATERIALS AND STRUCTURES. Kaspar Willam. Isotropic Elastic Models: Invariant vs Principal Formulations
MODELING OF CONCRETE MATERIALS AND STRUCTURES Kaspar Willam University of Colorado at Boulder Class Meeting #2: Nonlinear Elastic Models Isotropic Elastic Models: Invariant vs Principal Formulations Elastic
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationThe Relationship between the Applied Torque and Stresses in PostTension Structures
ECNDT 6  Poster 218 The Relationship between the Applied Torque and Stresses in PostTension Structures Fui Kiew LIEW, Sinin HAMDAN * and Mohd. Shahril OSMAN, Faculty of Engineering, Universiti Malaysia
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationPrediction of Compressive Strength of Fibrous Composites Using Two Different Approaches
Jordan Journal of Civil Engineering, Volume 8, No. 2, 214 Prediction of Compressive Strength of Fibrous Composites Using Two Different Approaches Yousef S. Al Rjoub 1) * and Karim S. Numayr 2) 1) Civil
More informationSIMULATION OF PLANE STRAIN FIBER COMPOSITE PLATES IN BENDING THROUGH A BEM/ACA/HM FORMULATION
8 th GRACM International Congress on Computational Mechanics Volos, 12 July 15 July 2015 SIMULATION OF PLANE STRAIN FIBER COMPOSITE PLATES IN BENDING THROUGH A BEM/ACA/HM FORMULATION Theodore V. Gortsas
More informationDetermination of Poisson s Ratio of Rock Material by Changing Axial Stress and Unloading Lateral Stress Test
Rock Mech Rock Eng DOI 10.1007/s0060301405869 TECHNICAL NOTE Determination of Poisson s Ratio of Rock Material by Changing Axial Stress and Unloading Lateral Stress Test Xiangtao Xu Runqiu Huang Hua
More information1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine Spring 2004 LABORATORY ASSIGNMENT NUMBER 6
1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine MIT Spring 2004 LABORATORY ASSIGNMENT NUMBER 6 COMPRESSION TESTING AND ANISOTROPY OF WOOD Purpose: Reading: During this laboratory
More informationWheatstone Bridge Nonlinearity
Index: Nonlinearity Wheatstone Bridge Nonlinearity Introduction General Considerations The "Unbalanced" Circuit The Unbalanced Circuit Table of Contents Output & Nonlinearity with Various Bridge/Strain
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More information2.1 Strain energy functions for incompressible materials
Chapter 2 Strain energy functions The aims of constitutive theories are to develop mathematical models for representing the real behavior of matter, to determine the material response and in general, to
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationModeling of FiberReinforced Membrane Materials Daniel Balzani. (Acknowledgement: Anna Zahn) Tasks Week 2 Winter term 2014
Institute of echanics and Shell Structures Faculty Civil Engineering Chair of echanics odeling of FiberReinforced embrane aterials OOC@TU9 Daniel Balani (Acknowledgement: Anna Zahn Tasks Week 2 Winter
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More information